#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:55:54 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179431 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/28/4332876.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4332876
loop_
_publ_author_name
'Sun, Junliang'
'Yang, Min'
'Li, Guobao'
'Yang, Tao'
'Liao, Fuhui'
'Wang, Yingxia'
'Xiong, Ming'
'Lin, Jianhua'
_publ_section_title
;
 New Barium Cobaltite Series Ban+1ConO3n+3(Co8O8):  Intergrowth
 Structure Containing Perovskite and CdI2-Type Layers
;
_journal_issue                   23
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9151
_journal_page_last               9153
_journal_paper_doi               10.1021/ic060992v
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Ba3 Co10 O17'
_chemical_formula_weight         1273.29
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            3
_cell_length_a                   5.6901(4)
_cell_length_b                   5.6901(4)
_cell_length_c                   35.937(5)
_cell_measurement_temperature    296(2)
_cell_volume                     1007.66(17)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.957
_diffrn_measured_fraction_theta_max 0.957
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0506
_diffrn_reflns_av_sigmaI/netI    0.0434
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       54
_diffrn_reflns_limit_l_min       -44
_diffrn_reflns_number            2859
_diffrn_reflns_theta_full        33.36
_diffrn_reflns_theta_max         33.36
_diffrn_reflns_theta_min         3.40
_exptl_absorpt_coefficient_mu    20.722
_exptl_absorpt_correction_T_max  0.357
_exptl_absorpt_correction_T_min  0.095
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2001)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.295
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       sheet
_exptl_crystal_F_000             1722
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.05
_refine_diff_density_max         3.095
_refine_diff_density_min         -3.291
_refine_diff_density_rms         0.541
_refine_ls_extinction_coef       0.00056(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.006
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     39
_refine_ls_number_reflns         532
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.006
_refine_ls_R_factor_all          0.0449
_refine_ls_R_factor_gt           0.0421
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0698P)²+36.1768P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1103
_refine_ls_wR_factor_ref         0.1127
_reflns_number_gt                485
_reflns_number_total             532
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic060992vsup2.cif
_cod_data_source_block           r-3mlast
_cod_original_cell_volume        1007.65(18)
_cod_original_sg_symbol_H-M      R-3m:H
_cod_database_code               4332876
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.0000 0.0000 0.0000 0.0109(3) Uani 1 12 d S
Ba2 Ba 0.6667 0.3333 0.93188(2) 0.0096(2) Uani 1 6 d S
Co1 Co 0.3333 0.6667 0.1667 0.0067(4) Uani 1 12 d S
Co2 Co 0.8333 0.1667 0.1667 0.0051(3) Uani 1 4 d S
Co3 Co 0.0000 0.0000 0.30605(5) 0.0083(3) Uani 1 6 d S
Co4 Co 0.0000 0.0000 0.23147(5) 0.0058(3) Uani 1 6 d S
Co5 Co 0.6667 0.3333 0.24519(5) 0.0075(3) Uani 1 6 d S
O1 O 0.6920(9) -0.1540(5) 0.19704(12) 0.0057(7) Uani 1 2 d S
O2 O 0.0000 0.0000 0.1400(2) 0.0057(7) Uani 1 6 d S
O3 O 0.4877(5) 0.5123(5) 0.40230(13) 0.0088(9) Uani 1 2 d S
O4 O 0.5000 0.5000 0.0000 0.0120(13) Uani 1 4 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Ba1 O4 180.0 1_445 .
O4 Ba1 O4 120.0 1_445 3_565
O4 Ba1 O4 60.0 . 3_565
O4 Ba1 O4 60.0 1_445 3
O4 Ba1 O4 120.0 . 3
O4 Ba1 O4 180.0 3_565 3
O4 Ba1 O4 120.0 1_445 2_655
O4 Ba1 O4 60.0 . 2_655
O4 Ba1 O4 120.0 3_565 2_655
O4 Ba1 O4 60.0 3 2_655
O4 Ba1 O4 60.0 1_445 2
O4 Ba1 O4 120.0 . 2
O4 Ba1 O4 60.0 3_565 2
O4 Ba1 O4 120.0 3 2
O4 Ba1 O4 180.0 2_655 2
O4 Ba1 O3 90.0 1_445 13_444
O4 Ba1 O3 90.0 . 13_444
O4 Ba1 O3 59.85(7) 3_565 13_444
O4 Ba1 O3 120.15(7) 3 13_444
O4 Ba1 O3 120.15(7) 2_655 13_444
O4 Ba1 O3 59.85(7) 2 13_444
O4 Ba1 O3 90.0 1_445 25
O4 Ba1 O3 90.0 . 25
O4 Ba1 O3 120.15(7) 3_565 25
O4 Ba1 O3 59.85(7) 3 25
O4 Ba1 O3 59.85(7) 2_655 25
O4 Ba1 O3 120.15(7) 2 25
O3 Ba1 O3 180.00(10) 13_444 25
O4 Ba1 O3 59.85(7) 1_445 27_445
O4 Ba1 O3 120.15(7) . 27_445
O4 Ba1 O3 90.0 3_565 27_445
O4 Ba1 O3 90.0 3 27_445
O4 Ba1 O3 120.15(7) 2_655 27_445
O4 Ba1 O3 59.85(7) 2 27_445
O3 Ba1 O3 119.71(15) 13_444 27_445
O3 Ba1 O3 60.29(15) 25 27_445
O4 Ba1 O3 120.15(7) 1_445 15_554
O4 Ba1 O3 59.85(7) . 15_554
O4 Ba1 O3 90.0 3_565 15_554
O4 Ba1 O3 90.0 3 15_554
O4 Ba1 O3 59.85(7) 2_655 15_554
O4 Ba1 O3 120.15(7) 2 15_554
O3 Ba1 O3 60.29(15) 13_444 15_554
O3 Ba1 O3 119.71(15) 25 15_554
O3 Ba1 O3 180.00(15) 27_445 15_554
O4 Ba1 O3 120.15(7) 1_445 26_455
O4 Ba1 O3 59.85(7) . 26_455
O4 Ba1 O3 59.85(7) 3_565 26_455
O4 Ba1 O3 120.15(7) 3 26_455
O4 Ba1 O3 90.0 2_655 26_455
O4 Ba1 O3 90.0 2 26_455
O3 Ba1 O3 119.71(15) 13_444 26_455
O3 Ba1 O3 60.29(15) 25 26_455
O3 Ba1 O3 60.29(15) 27_445 26_455
O3 Ba1 O3 119.71(15) 15_554 26_455
O4 Ba1 O3 59.85(7) 1_445 14_544
O4 Ba1 O3 120.15(7) . 14_544
O4 Ba1 O3 120.15(7) 3_565 14_544
O4 Ba1 O3 59.85(7) 3 14_544
O4 Ba1 O3 90.0 2_655 14_544
O4 Ba1 O3 90.0 2 14_544
O3 Ba1 O3 60.29(15) 13_444 14_544
O3 Ba1 O3 119.71(15) 25 14_544
O3 Ba1 O3 119.71(15) 27_445 14_544
O3 Ba1 O3 60.29(15) 15_554 14_544
O3 Ba1 O3 180.0(2) 26_455 14_544
O3 Ba2 O3 64.89(19) 27_546 26_556
O3 Ba2 O3 119.990(5) 27_546 25_666
O3 Ba2 O3 55.11(19) 26_556 25_666
O3 Ba2 O3 55.11(19) 27_546 25_556
O3 Ba2 O3 119.990(5) 26_556 25_556
O3 Ba2 O3 174.96(18) 25_666 25_556
O3 Ba2 O3 175.0(2) 27_546 27_556
O3 Ba2 O3 119.989(12) 26_556 27_556
O3 Ba2 O3 64.89(19) 25_666 27_556
O3 Ba2 O3 119.988(7) 25_556 27_556
O3 Ba2 O3 119.989(11) 27_546 26_456
O3 Ba2 O3 175.0(2) 26_556 26_456
O3 Ba2 O3 119.988(7) 25_666 26_456
O3 Ba2 O3 64.89(19) 25_556 26_456
O3 Ba2 O3 55.11(19) 27_556 26_456
O3 Ba2 O4 91.87(9) 27_546 3_666
O3 Ba2 O4 60.98(10) 26_556 3_666
O3 Ba2 O4 60.98(10) 25_666 3_666
O3 Ba2 O4 118.62(10) 25_556 3_666
O3 Ba2 O4 91.87(9) 27_556 3_666
O3 Ba2 O4 118.62(10) 26_456 3_666
O3 Ba2 O4 60.98(10) 27_546 2_656
O3 Ba2 O4 91.87(9) 26_556 2_656
O3 Ba2 O4 118.62(10) 25_666 2_656
O3 Ba2 O4 60.98(10) 25_556 2_656
O3 Ba2 O4 118.62(10) 27_556 2_656
O3 Ba2 O4 91.87(9) 26_456 2_656
O4 Ba2 O4 57.700(15) 3_666 2_656
O3 Ba2 O4 118.62(10) 27_546 1_556
O3 Ba2 O4 118.62(10) 26_556 1_556
O3 Ba2 O4 91.87(9) 25_666 1_556
O3 Ba2 O4 91.87(9) 25_556 1_556
O3 Ba2 O4 60.98(10) 27_556 1_556
O3 Ba2 O4 60.98(10) 26_456 1_556
O4 Ba2 O4 57.700(15) 3_666 1_556
O4 Ba2 O4 57.700(15) 2_656 1_556
O3 Ba2 O1 119.02(12) 27_546 14_545
O3 Ba2 O1 119.02(12) 26_556 14_545
O3 Ba2 O1 90.94(10) 25_666 14_545
O3 Ba2 O1 90.94(10) 25_556 14_545
O3 Ba2 O1 58.18(12) 27_556 14_545
O3 Ba2 O1 58.18(12) 26_456 14_545
O4 Ba2 O1 146.76(4) 3_666 14_545
O4 Ba2 O1 146.76(4) 2_656 14_545
O4 Ba2 O1 110.33(8) 1_556 14_545
O3 Ba2 O1 58.18(11) 27_546 15_655
O3 Ba2 O1 90.94(10) 26_556 15_655
O3 Ba2 O1 119.02(12) 25_666 15_655
O3 Ba2 O1 58.18(12) 25_556 15_655
O3 Ba2 O1 119.02(12) 27_556 15_655
O3 Ba2 O1 90.94(10) 26_456 15_655
O4 Ba2 O1 146.76(4) 3_666 15_655
O4 Ba2 O1 110.33(9) 2_656 15_655
O4 Ba2 O1 146.76(4) 1_556 15_655
O1 Ba2 O1 60.89(14) 14_545 15_655
O3 Ba2 O1 90.94(10) 27_546 13
O3 Ba2 O1 58.18(11) 26_556 13
O3 Ba2 O1 58.18(12) 25_666 13
O3 Ba2 O1 119.02(12) 25_556 13
O3 Ba2 O1 90.94(10) 27_556 13
O3 Ba2 O1 119.02(12) 26_456 13
O4 Ba2 O1 110.33(9) 3_666 13
O4 Ba2 O1 146.76(4) 2_656 13
O4 Ba2 O1 146.76(4) 1_556 13
O1 Ba2 O1 60.89(14) 14_545 13
O1 Ba2 O1 60.89(14) 15_655 13
O1 Co1 O1 94.93(16) 26_565 25
O1 Co1 O1 94.93(16) 26_565 27_455
O1 Co1 O1 94.93(16) 25 27_455
O1 Co1 O1 180.0 26_565 2
O1 Co1 O1 85.07(16) 25 2
O1 Co1 O1 85.07(16) 27_455 2
O1 Co1 O1 85.07(16) 26_565 1_565
O1 Co1 O1 179.998(1) 25 1_565
O1 Co1 O1 85.07(16) 27_455 1_565
O1 Co1 O1 94.93(16) 2 1_565
O1 Co1 O1 85.07(16) 26_565 3_665
O1 Co1 O1 85.07(16) 25 3_665
O1 Co1 O1 179.998(1) 27_455 3_665
O1 Co1 O1 94.93(16) 2 3_665
O1 Co1 O1 94.93(16) 1_565 3_665
O1 Co1 Co2 90.0 26_565 1_455
O1 Co1 Co2 42.53(8) 25 1_455
O1 Co1 Co2 137.47(8) 27_455 1_455
O1 Co1 Co2 90.0 2 1_455
O1 Co1 Co2 137.47(8) 1_565 1_455
O1 Co1 Co2 42.53(8) 3_665 1_455
O1 Co1 Co2 137.47(8) 26_565 2
O1 Co1 Co2 42.53(8) 25 2
O1 Co1 Co2 90.0 27_455 2
O1 Co1 Co2 42.53(8) 2 2
O1 Co1 Co2 137.47(8) 1_565 2
O1 Co1 Co2 90.0 3_665 2
Co2 Co1 Co2 60.0 1_455 2
O1 Co1 Co2 90.0 26_565 1_565
O1 Co1 Co2 137.47(8) 25 1_565
O1 Co1 Co2 42.53(8) 27_455 1_565
O1 Co1 Co2 90.0 2 1_565
O1 Co1 Co2 42.53(8) 1_565 1_565
O1 Co1 Co2 137.47(8) 3_665 1_565
Co2 Co1 Co2 180.0 1_455 1_565
Co2 Co1 Co2 120.0 2 1_565
O1 Co1 Co2 137.47(8) 26_565 3_675
O1 Co1 Co2 90.0 25 3_675
O1 Co1 Co2 42.53(8) 27_455 3_675
O1 Co1 Co2 42.53(8) 2 3_675
O1 Co1 Co2 90.0 1_565 3_675
O1 Co1 Co2 137.47(8) 3_665 3_675
Co2 Co1 Co2 120.0 1_455 3_675
Co2 Co1 Co2 60.0 2 3_675
Co2 Co1 Co2 60.0 1_565 3_675
O1 Co1 Co2 42.53(8) 26_565 3_665
O1 Co1 Co2 90.0 25 3_665
O1 Co1 Co2 137.47(8) 27_455 3_665
O1 Co1 Co2 137.47(8) 2 3_665
O1 Co1 Co2 90.0 1_565 3_665
O1 Co1 Co2 42.53(8) 3_665 3_665
Co2 Co1 Co2 60.0 1_455 3_665
Co2 Co1 Co2 120.0 2 3_665
Co2 Co1 Co2 120.0 1_565 3_665
Co2 Co1 Co2 180.0 3_675 3_665
O1 Co1 Co2 42.53(8) 26_565 2_655
O1 Co1 Co2 137.47(8) 25 2_655
O1 Co1 Co2 90.0 27_455 2_655
O1 Co1 Co2 137.47(8) 2 2_655
O1 Co1 Co2 42.53(8) 1_565 2_655
O1 Co1 Co2 90.0 3_665 2_655
Co2 Co1 Co2 120.0 1_455 2_655
Co2 Co1 Co2 180.0 2 2_655
Co2 Co1 Co2 60.0 1_565 2_655
Co2 Co1 Co2 120.0 3_675 2_655
Co2 Co1 Co2 60.0 3_665 2_655
O2 Co2 O2 179.998(1) 1_655 25
O2 Co2 O1 96.34(19) 1_655 27_445
O2 Co2 O1 83.66(19) 25 27_445
O2 Co2 O1 96.34(19) 1_655 25_655
O2 Co2 O1 83.66(19) 25 25_655
O1 Co2 O1 86.2(3) 27_445 25_655
O2 Co2 O1 83.66(19) 1_655 3_765
O2 Co2 O1 96.34(19) 25 3_765
O1 Co2 O1 179.997(1) 27_445 3_765
O1 Co2 O1 93.8(3) 25_655 3_765
O2 Co2 O1 83.66(19) 1_655 .
O2 Co2 O1 96.34(19) 25 .
O1 Co2 O1 93.8(3) 27_445 .
O1 Co2 O1 179.997(1) 25_655 .
O1 Co2 O1 86.2(3) 3_765 .
O2 Co2 Co4 94.9(2) 1_655 25
O2 Co2 Co4 85.1(2) 25 25
O1 Co2 Co4 43.24(13) 27_445 25
O1 Co2 Co4 43.24(13) 25_655 25
O1 Co2 Co4 136.77(13) 3_765 25
O1 Co2 Co4 136.77(13) . 25
O2 Co2 Co4 85.1(2) 1_655 1_655
O2 Co2 Co4 94.9(2) 25 1_655
O1 Co2 Co4 136.76(13) 27_445 1_655
O1 Co2 Co4 136.76(13) 25_655 1_655
O1 Co2 Co4 43.23(13) 3_765 1_655
O1 Co2 Co4 43.23(13) . 1_655
Co4 Co2 Co4 180.0 25 1_655
O2 Co2 Co2 138.39(15) 1_655 3_665
O2 Co2 Co2 41.61(15) 25 3_665
O1 Co2 Co2 42.30(10) 27_445 3_665
O1 Co2 Co2 86.77(12) 25_655 3_665
O1 Co2 Co2 137.69(10) 3_765 3_665
O1 Co2 Co2 93.23(12) . 3_665
Co4 Co2 Co2 60.055(16) 25 3_665
Co4 Co2 Co2 119.944(16) 1_655 3_665
O2 Co2 Co2 138.39(15) 1_655 2_655
O2 Co2 Co2 41.61(15) 25 2_655
O1 Co2 Co2 86.77(12) 27_445 2_655
O1 Co2 Co2 42.30(10) 25_655 2_655
O1 Co2 Co2 93.23(12) 3_765 2_655
O1 Co2 Co2 137.69(10) . 2_655
Co4 Co2 Co2 60.055(16) 25 2_655
Co4 Co2 Co2 119.944(16) 1_655 2_655
Co2 Co2 Co2 60.0 3_665 2_655
O2 Co2 Co1 90.0 1_655 1_655
O2 Co2 Co1 90.0 25 1_655
O1 Co2 Co1 133.10(13) 27_445 1_655
O1 Co2 Co1 46.90(13) 25_655 1_655
O1 Co2 Co1 46.90(13) 3_765 1_655
O1 Co2 Co1 133.10(13) . 1_655
Co4 Co2 Co1 90.0 25 1_655
Co4 Co2 Co1 90.0 1_655 1_655
Co2 Co2 Co1 120.0 3_665 1_655
Co2 Co2 Co1 60.0 2_655 1_655
O2 Co2 Co1 90.0 1_655 1_545
O2 Co2 Co1 90.0 25 1_545
O1 Co2 Co1 46.90(13) 27_445 1_545
O1 Co2 Co1 133.10(13) 25_655 1_545
O1 Co2 Co1 133.10(13) 3_765 1_545
O1 Co2 Co1 46.90(13) . 1_545
Co4 Co2 Co1 90.0 25 1_545
Co4 Co2 Co1 90.0 1_655 1_545
Co2 Co2 Co1 60.0 3_665 1_545
Co2 Co2 Co1 120.0 2_655 1_545
Co1 Co2 Co1 180.0 1_655 1_545
O4 Co3 O4 96.07(6) 7_445 8
O4 Co3 O4 96.08(6) 7_445 9_455
O4 Co3 O4 96.07(6) 8 9_455
O4 Co3 O3 166.28(15) 7_445 31
O4 Co3 O3 93.08(8) 8 31
O4 Co3 O3 93.08(8) 9_455 31
O4 Co3 O3 93.08(8) 7_445 32_445
O4 Co3 O3 166.28(15) 8 32_445
O4 Co3 O3 93.08(8) 9_455 32_445
O3 Co3 O3 76.2(2) 31 32_445
O4 Co3 O3 93.08(8) 7_445 33_545
O4 Co3 O3 93.08(8) 8 33_545
O4 Co3 O3 166.28(15) 9_455 33_545
O3 Co3 O3 76.2(2) 31 33_545
O3 Co3 O3 76.2(2) 32_445 33_545
O4 Co3 Co4 120.84(5) 7_445 .
O4 Co3 Co4 120.84(5) 8 .
O4 Co3 Co4 120.84(5) 9_455 .
O3 Co3 Co4 45.44(13) 31 .
O3 Co3 Co4 45.44(13) 32_445 .
O3 Co3 Co4 45.44(13) 33_545 .
O4 Co3 Ba1 56.083(13) 7_445 7
O4 Co3 Ba1 56.083(13) 8 7
O4 Co3 Ba1 132.54(7) 9_455 7
O3 Co3 Ba1 122.83(3) 31 7
O3 Co3 Ba1 122.83(3) 32_445 7
O3 Co3 Ba1 61.18(12) 33_545 7
Co4 Co3 Ba1 106.62(3) . 7
O4 Co3 Ba1 56.083(13) 7_445 7_445
O4 Co3 Ba1 132.54(7) 8 7_445
O4 Co3 Ba1 56.083(13) 9_455 7_445
O3 Co3 Ba1 122.82(3) 31 7_445
O3 Co3 Ba1 61.18(12) 32_445 7_445
O3 Co3 Ba1 122.83(3) 33_545 7_445
Co4 Co3 Ba1 106.62(3) . 7_445
Ba1 Co3 Ba1 112.17(3) 7 7_445
O4 Co3 Ba1 132.54(7) 7_445 7_455
O4 Co3 Ba1 56.082(13) 8 7_455
O4 Co3 Ba1 56.082(13) 9_455 7_455
O3 Co3 Ba1 61.18(12) 31 7_455
O3 Co3 Ba1 122.83(3) 32_445 7_455
O3 Co3 Ba1 122.83(3) 33_545 7_455
Co4 Co3 Ba1 106.62(3) . 7_455
Ba1 Co3 Ba1 112.16(3) 7 7_455
Ba1 Co3 Ba1 112.16(3) 7_445 7_455
O4 Co3 Ba2 59.16(5) 7_445 25_556
O4 Co3 Ba2 59.16(5) 8 25_556
O4 Co3 Ba2 59.16(5) 9_455 25_556
O3 Co3 Ba2 134.56(13) 31 25_556
O3 Co3 Ba2 134.56(13) 32_445 25_556
O3 Co3 Ba2 134.56(13) 33_545 25_556
Co4 Co3 Ba2 180.0 . 25_556
Ba1 Co3 Ba2 73.38(3) 7 25_556
Ba1 Co3 Ba2 73.38(3) 7_445 25_556
Ba1 Co3 Ba2 73.38(3) 7_455 25_556
O4 Co3 Ba2 54.91(2) 7_445 7_444
O4 Co3 Ba2 126.946(6) 8 7_444
O4 Co3 Ba2 126.946(6) 9_455 7_444
O3 Co3 Ba2 111.37(14) 31 7_444
O3 Co3 Ba2 52.305(17) 32_445 7_444
O3 Co3 Ba2 52.305(17) 33_545 7_444
Co4 Co3 Ba2 65.93(3) . 7_444
Ba1 Co3 Ba2 71.290(7) 7 7_444
Ba1 Co3 Ba2 71.290(7) 7_445 7_444
Ba1 Co3 Ba2 172.55(6) 7_455 7_444
Ba2 Co3 Ba2 114.07(3) 25_556 7_444
O3 Co4 O3 86.3(2) 31 33_545
O3 Co4 O3 86.3(2) 31 32_445
O3 Co4 O3 86.3(2) 33_545 32_445
O3 Co4 O1 94.69(14) 31 1_455
O3 Co4 O1 178.7(2) 33_545 1_455
O3 Co4 O1 94.69(14) 32_445 1_455
O3 Co4 O1 178.7(2) 31 2_545
O3 Co4 O1 94.69(14) 33_545 2_545
O3 Co4 O1 94.69(14) 32_445 2_545
O1 Co4 O1 84.3(2) 1_455 2_545
O3 Co4 O1 94.69(14) 31 3_665
O3 Co4 O1 94.69(14) 33_545 3_665
O3 Co4 O1 178.7(2) 32_445 3_665
O1 Co4 O1 84.3(2) 1_455 3_665
O1 Co4 O1 84.3(2) 2_545 3_665
O3 Co4 Co3 52.15(15) 31 .
O3 Co4 Co3 52.15(15) 33_545 .
O3 Co4 Co3 52.15(15) 32_445 .
O1 Co4 Co3 129.19(14) 1_455 .
O1 Co4 Co3 129.19(14) 2_545 .
O1 Co4 Co3 129.19(14) 3_665 .
O3 Co4 Co2 136.80(10) 31 2_545
O3 Co4 Co2 136.80(10) 33_545 2_545
O3 Co4 Co2 92.66(15) 32_445 2_545
O1 Co4 Co2 42.29(9) 1_455 2_545
O1 Co4 Co2 42.29(9) 2_545 2_545
O1 Co4 Co2 86.00(14) 3_665 2_545
Co3 Co4 Co2 144.805(19) . 2_545
O3 Co4 Co2 92.66(15) 31 1_455
O3 Co4 Co2 136.80(10) 33_545 1_455
O3 Co4 Co2 136.80(10) 32_445 1_455
O1 Co4 Co2 42.29(9) 1_455 1_455
O1 Co4 Co2 86.00(14) 2_545 1_455
O1 Co4 Co2 42.29(9) 3_665 1_455
Co3 Co4 Co2 144.805(19) . 1_455
Co2 Co4 Co2 59.89(3) 2_545 1_455
O3 Co4 Co2 136.80(10) 31 3_665
O3 Co4 Co2 92.66(15) 33_545 3_665
O3 Co4 Co2 136.80(10) 32_445 3_665
O1 Co4 Co2 86.00(14) 1_455 3_665
O1 Co4 Co2 42.29(9) 2_545 3_665
O1 Co4 Co2 42.29(9) 3_665 3_665
Co3 Co4 Co2 144.805(19) . 3_665
Co2 Co4 Co2 59.89(3) 2_545 3_665
Co2 Co4 Co2 59.89(3) 1_455 3_665
O3 Co4 Ba2 121.89(16) 31 7_444
O3 Co4 Ba2 54.349(14) 33_545 7_444
O3 Co4 Ba2 54.349(14) 32_445 7_444
O1 Co4 Ba2 125.616(17) 1_455 7_444
O1 Co4 Ba2 59.45(13) 2_545 7_444
O1 Co4 Ba2 125.616(18) 3_665 7_444
Co3 Co4 Ba2 69.74(3) . 7_444
Co2 Co4 Ba2 90.722(15) 2_545 7_444
Co2 Co4 Ba2 145.45(4) 1_455 7_444
Co2 Co4 Ba2 90.722(15) 3_665 7_444
O3 Co4 Ba2 54.349(14) 31 7_454
O3 Co4 Ba2 54.350(14) 33_545 7_454
O3 Co4 Ba2 121.89(16) 32_445 7_454
O1 Co4 Ba2 125.615(17) 1_455 7_454
O1 Co4 Ba2 125.616(18) 2_545 7_454
O1 Co4 Ba2 59.45(13) 3_665 7_454
Co3 Co4 Ba2 69.74(3) . 7_454
Co2 Co4 Ba2 145.45(4) 2_545 7_454
Co2 Co4 Ba2 90.721(15) 1_455 7_454
Co2 Co4 Ba2 90.722(15) 3_665 7_454
Ba2 Co4 Ba2 108.67(3) 7_444 7_454
O2 Co5 O3 111.33(15) 25 32
O2 Co5 O3 111.33(15) 25 33_545
O3 Co5 O3 107.55(16) 32 33_545
O2 Co5 O3 111.34(15) 25 31_655
O3 Co5 O3 107.54(16) 32 31_655
O3 Co5 O3 107.54(16) 33_545 31_655
O2 Co5 Ba1 180.0 25 7
O3 Co5 Ba1 68.66(15) 32 7
O3 Co5 Ba1 68.66(15) 33_545 7
O3 Co5 Ba1 68.67(15) 31_655 7
O2 Co5 Ba2 102.35(3) 25 7_554
O3 Co5 Ba2 57.805(11) 32 7_554
O3 Co5 Ba2 146.31(16) 33_545 7_554
O3 Co5 Ba2 57.807(10) 31_655 7_554
Ba1 Co5 Ba2 77.65(3) 7 7_554
O2 Co5 Ba2 102.35(3) 25 7_444
O3 Co5 Ba2 146.31(16) 32 7_444
O3 Co5 Ba2 57.805(11) 33_545 7_444
O3 Co5 Ba2 57.807(11) 31_655 7_444
Ba1 Co5 Ba2 77.65(3) 7 7_444
Ba2 Co5 Ba2 115.55(2) 7_554 7_444
O2 Co5 Ba2 102.35(3) 25 7_454
O3 Co5 Ba2 57.807(10) 32 7_454
O3 Co5 Ba2 57.807(10) 33_545 7_454
O3 Co5 Ba2 146.31(16) 31_655 7_454
Ba1 Co5 Ba2 77.65(3) 7 7_454
Ba2 Co5 Ba2 115.55(2) 7_554 7_454
Ba2 Co5 Ba2 115.55(2) 7_444 7_454
Co2 O1 Co2 95.4(2) 2_645 .
Co2 O1 Co4 94.48(16) 2_645 1_655
Co2 O1 Co4 94.48(16) . 1_655
Co2 O1 Co1 90.56(16) 2_645 1_545
Co2 O1 Co1 90.56(16) . 1_545
Co4 O1 Co1 172.5(3) 1_655 1_545
Co2 O1 Ba2 132.22(10) 2_645 7_444
Co2 O1 Ba2 132.22(10) . 7_444
Co4 O1 Ba2 86.62(16) 1_655 7_444
Co1 O1 Ba2 85.88(14) 1_545 7_444
Co5 O2 Co2 120.3(2) 25 3_665
Co5 O2 Co2 120.3(2) 25 2_545
Co2 O2 Co2 96.8(3) 3_665 2_545
Co5 O2 Co2 120.3(2) 25 1_455
Co2 O2 Co2 96.8(3) 3_665 1_455
Co2 O2 Co2 96.8(3) 2_545 1_455
Co5 O3 Co4 120.8(3) 31_655 31
Co5 O3 Co3 156.8(3) 31_655 31
Co4 O3 Co3 82.41(18) 31 31
Co5 O3 Ba2 87.94(10) 31_655 25_556
Co4 O3 Ba2 92.30(9) 31 25_556
Co3 O3 Ba2 91.32(10) 31 25_556
Co5 O3 Ba2 87.94(10) 31_655 25_666
Co4 O3 Ba2 92.30(9) 31 25_666
Co3 O3 Ba2 91.32(10) 31 25_666
Ba2 O3 Ba2 174.96(19) 25_556 25_666
Co5 O3 Ba1 75.89(15) 31_655 7
Co4 O3 Ba1 163.3(2) 31 7
Co3 O3 Ba1 80.88(15) 31 7
Ba2 O3 Ba1 88.09(9) 25_556 7
Ba2 O3 Ba1 88.09(9) 25_666 7
Co3 O4 Co3 180.00(9) 25 13_554
Co3 O4 Ba1 90.0 25 .
Co3 O4 Ba1 90.0 13_554 .
Co3 O4 Ba1 90.0 25 1_665
Co3 O4 Ba1 90.0 13_554 1_665
Ba1 O4 Ba1 180.0 . 1_665
Co3 O4 Ba2 86.98(5) 25 1_554
Co3 O4 Ba2 93.02(5) 13_554 1_554
Ba1 O4 Ba2 90.0 . 1_554
Ba1 O4 Ba2 90.0 1_665 1_554
Co3 O4 Ba2 93.02(5) 25 19_666
Co3 O4 Ba2 86.98(5) 13_554 19_666
Ba1 O4 Ba2 90.0 . 19_666
Ba1 O4 Ba2 90.0 1_665 19_666
Ba2 O4 Ba2 180.000(16) 1_554 19_666
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 O4 2.8451(2) 1_445
Ba1 O4 2.8451(2) .
Ba1 O4 2.8451(2) 3_565
Ba1 O4 2.8451(2) 3
Ba1 O4 2.8451(2) 2_655
Ba1 O4 2.8451(2) 2
Ba1 O3 3.042(5) 13_444
Ba1 O3 3.042(5) 25
Ba1 O3 3.042(5) 27_445
Ba1 O3 3.042(5) 15_554
Ba1 O3 3.042(5) 26_455
Ba1 O3 3.042(5) 14_544
Ba2 O3 2.848(2) 27_546
Ba2 O3 2.848(2) 26_556
Ba2 O3 2.848(3) 25_666
Ba2 O3 2.848(3) 25_556
Ba2 O3 2.848(3) 27_556
Ba2 O3 2.848(3) 26_456
Ba2 O4 2.9481(7) 3_666
Ba2 O4 2.9481(7) 2_656
Ba2 O4 2.9481(7) 1_556
Ba2 O1 3.021(4) 14_545
Ba2 O1 3.021(5) 15_655
Ba2 O1 3.021(5) 13
Co1 O1 2.077(4) 26_565
Co1 O1 2.077(4) 25
Co1 O1 2.077(4) 27_455
Co1 O1 2.077(4) 2
Co1 O1 2.077(4) 1_565
Co1 O1 2.077(4) 3_665
Co1 Co2 2.8451(2) 1_455
Co1 Co2 2.8451(2) 2
Co1 Co2 2.8451(2) 1_565
Co1 Co2 2.8451(2) 3_675
Co1 Co2 2.8451(2) 3_665
Co1 Co2 2.8451(2) 2_655
Co2 O2 1.902(4) 1_655
Co2 O2 1.903(4) 25
Co2 O1 1.923(3) 27_445
Co2 O1 1.923(3) 25_655
Co2 O1 1.923(3) 3_765
Co2 O1 1.923(3) .
Co2 Co4 2.8499(14) 25
Co2 Co4 2.8499(14) 1_655
Co2 Co2 2.8451(2) 3_665
Co2 Co2 2.8451(2) 2_655
Co2 Co1 2.8451(2) 1_655
Co2 Co1 2.8451(2) 1_545
Co3 O4 1.9131(9) 7_445
Co3 O4 1.9131(9) 8
Co3 O4 1.9131(9) 9_455
Co3 O3 2.135(5) 31
Co3 O3 2.135(5) 32_445
Co3 O3 2.135(5) 33_545
Co3 Co4 2.680(2) .
Co3 Ba1 3.4284(5) 7
Co3 Ba1 3.4284(6) 7_445
Co3 Ba1 3.4285(6) 7_455
Co3 Ba2 3.4288(19) 25_556
Co3 Ba2 3.5980(8) 7_444
Co4 O3 1.926(5) 31
Co4 O3 1.926(5) 33_545
Co4 O3 1.926(5) 32_445
Co4 O1 1.958(5) 1_455
Co4 O1 1.958(5) 2_545
Co4 O1 1.958(5) 3_665
Co4 Co2 2.8499(14) 2_545
Co4 Co2 2.8499(14) 1_455
Co4 Co2 2.8499(14) 3_665
Co4 Ba2 3.5018(6) 7_444
Co4 Ba2 3.5018(6) 7_454
Co5 O2 1.862(9) 25
Co5 O3 1.894(5) 32
Co5 O3 1.894(5) 33_545
Co5 O3 1.894(5) 31_655
Co5 Ba1 3.1676(17) 7
Co5 Ba2 3.3630(4) 7_554
Co5 Ba2 3.3630(4) 7_444
Co5 Ba2 3.3631(4) 7_454
O1 Co2 1.923(3) 2_645
O1 Co4 1.958(5) 1_655
O1 Co1 2.077(4) 1_545
O1 Ba2 3.021(4) 7_444
O2 Co5 1.862(9) 25
O2 Co2 1.902(4) 3_665
O2 Co2 1.902(4) 2_545
O2 Co2 1.902(4) 1_455
O3 Co5 1.894(5) 31_655
O3 Co4 1.926(5) 31
O3 Co3 2.135(5) 31
O3 Ba2 2.848(3) 25_556
O3 Ba2 2.848(3) 25_666
O3 Ba1 3.042(5) 7
O4 Co3 1.9131(9) 25
O4 Co3 1.9131(9) 13_554
O4 Ba1 2.8451(2) 1_665
O4 Ba2 2.9481(7) 1_554
O4 Ba2 2.9481(7) 19_666
